# Supplementary Information (SI) for Chemical Communications.
# This journal is © The Royal Society of Chemistry 2024

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_cc_163a_161b
_database_code_depnum_ccdc_archive 'CCDC 2356184'
loop_
_audit_author_name
_audit_author_address
'Leila Foroughi'
;University of Michigan
United States of America
;
_audit_update_record             
;
2024-07-30 deposited with the CCDC.	2024-08-01 downloaded from the CCDC.
;
_audit_creation_date             2024-05-10
_audit_creation_method           
;
Olex2 1.5-ac5-024
(compiled 2022.04.12 svn.rca3783a0 for Rigaku Oxford Diffraction, GUI svn.r6498)
;
_shelx_SHELXL_version_number     2018/3
loop_
_audit_author_email
matzger@umich.edu
careycy@umich.edu
foroug@umich.edu
_chemical_name_systematic        IRMOF-10
_chemical_name_common            IRMOF-10
_chemical_formula_moiety         'C42 H24 O13 Zn4'
_chemical_formula_sum            'C42 H24 O13 Zn4'
_chemical_formula_weight         998.09
_chemical_melting_point          ?
_exptl_crystal_description       'rhombic dodecahedral'
_exptl_crystal_colour            'clear light colourless'
_diffrn_ambient_temperature      293(2)
_chemical_oxdiff_formula         'C42 H24 O13 Zn4 '
_chemical_oxdiff_usercomment     'exchanged in hexanes'
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0181 0.0091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn -1.5491 0.6778 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      cubic
_space_group_IT_number           225
_space_group_name_H-M_alt        'F m -3 m'
_space_group_name_Hall           '-F 4 2 3'
_chemical_absolute_configuration ?
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, -z'
'-y, -x, -z'
'y, -x, z'
'-y, x, z'
'x, z, -y'
'-x, z, y'
'-x, -z, -y'
'x, -z, y'
'z, y, -x'
'z, -y, x'
'-z, y, x'
'-z, -y, -x'
'x, y+1/2, z+1/2'
'-x, -y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y+1/2, -z+1/2'
'z, x+1/2, y+1/2'
'z, -x+1/2, -y+1/2'
'-z, -x+1/2, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z+1/2, x+1/2'
'-y, z+1/2, -x+1/2'
'y, -z+1/2, -x+1/2'
'-y, -z+1/2, x+1/2'
'y, x+1/2, -z+1/2'
'-y, -x+1/2, -z+1/2'
'y, -x+1/2, z+1/2'
'-y, x+1/2, z+1/2'
'x, z+1/2, -y+1/2'
'-x, z+1/2, y+1/2'
'-x, -z+1/2, -y+1/2'
'x, -z+1/2, y+1/2'
'z, y+1/2, -x+1/2'
'z, -y+1/2, x+1/2'
'-z, y+1/2, x+1/2'
'-z, -y+1/2, -x+1/2'
'x+1/2, y, z+1/2'
'-x+1/2, -y, z+1/2'
'-x+1/2, y, -z+1/2'
'x+1/2, -y, -z+1/2'
'z+1/2, x, y+1/2'
'z+1/2, -x, -y+1/2'
'-z+1/2, -x, y+1/2'
'-z+1/2, x, -y+1/2'
'y+1/2, z, x+1/2'
'-y+1/2, z, -x+1/2'
'y+1/2, -z, -x+1/2'
'-y+1/2, -z, x+1/2'
'y+1/2, x, -z+1/2'
'-y+1/2, -x, -z+1/2'
'y+1/2, -x, z+1/2'
'-y+1/2, x, z+1/2'
'x+1/2, z, -y+1/2'
'-x+1/2, z, y+1/2'
'-x+1/2, -z, -y+1/2'
'x+1/2, -z, y+1/2'
'z+1/2, y, -x+1/2'
'z+1/2, -y, x+1/2'
'-z+1/2, y, x+1/2'
'-z+1/2, -y, -x+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'z+1/2, x+1/2, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x+1/2, y'
'-z+1/2, x+1/2, -y'
'y+1/2, z+1/2, x'
'-y+1/2, z+1/2, -x'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z+1/2, x'
'y+1/2, x+1/2, -z'
'-y+1/2, -x+1/2, -z'
'y+1/2, -x+1/2, z'
'-y+1/2, x+1/2, z'
'x+1/2, z+1/2, -y'
'-x+1/2, z+1/2, y'
'-x+1/2, -z+1/2, -y'
'x+1/2, -z+1/2, y'
'z+1/2, y+1/2, -x'
'z+1/2, -y+1/2, x'
'-z+1/2, y+1/2, x'
'-z+1/2, -y+1/2, -x'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-y, -x, z'
'y, x, z'
'-y, x, -z'
'y, -x, -z'
'-x, -z, y'
'x, -z, -y'
'x, z, y'
'-x, z, -y'
'-z, -y, x'
'-z, y, -x'
'z, -y, -x'
'z, y, x'
'-x, -y+1/2, -z+1/2'
'x, y+1/2, -z+1/2'
'x, -y+1/2, z+1/2'
'-x, y+1/2, z+1/2'
'-z, -x+1/2, -y+1/2'
'-z, x+1/2, y+1/2'
'z, x+1/2, -y+1/2'
'z, -x+1/2, y+1/2'
'-y, -z+1/2, -x+1/2'
'y, -z+1/2, x+1/2'
'-y, z+1/2, x+1/2'
'y, z+1/2, -x+1/2'
'-y, -x+1/2, z+1/2'
'y, x+1/2, z+1/2'
'-y, x+1/2, -z+1/2'
'y, -x+1/2, -z+1/2'
'-x, -z+1/2, y+1/2'
'x, -z+1/2, -y+1/2'
'x, z+1/2, y+1/2'
'-x, z+1/2, -y+1/2'
'-z, -y+1/2, x+1/2'
'-z, y+1/2, -x+1/2'
'z, -y+1/2, -x+1/2'
'z, y+1/2, x+1/2'
'-x+1/2, -y, -z+1/2'
'x+1/2, y, -z+1/2'
'x+1/2, -y, z+1/2'
'-x+1/2, y, z+1/2'
'-z+1/2, -x, -y+1/2'
'-z+1/2, x, y+1/2'
'z+1/2, x, -y+1/2'
'z+1/2, -x, y+1/2'
'-y+1/2, -z, -x+1/2'
'y+1/2, -z, x+1/2'
'-y+1/2, z, x+1/2'
'y+1/2, z, -x+1/2'
'-y+1/2, -x, z+1/2'
'y+1/2, x, z+1/2'
'-y+1/2, x, -z+1/2'
'y+1/2, -x, -z+1/2'
'-x+1/2, -z, y+1/2'
'x+1/2, -z, -y+1/2'
'x+1/2, z, y+1/2'
'-x+1/2, z, -y+1/2'
'-z+1/2, -y, x+1/2'
'-z+1/2, y, -x+1/2'
'z+1/2, -y, -x+1/2'
'z+1/2, y, x+1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, z'
'-z+1/2, -x+1/2, -y'
'-z+1/2, x+1/2, y'
'z+1/2, x+1/2, -y'
'z+1/2, -x+1/2, y'
'-y+1/2, -z+1/2, -x'
'y+1/2, -z+1/2, x'
'-y+1/2, z+1/2, x'
'y+1/2, z+1/2, -x'
'-y+1/2, -x+1/2, z'
'y+1/2, x+1/2, z'
'-y+1/2, x+1/2, -z'
'y+1/2, -x+1/2, -z'
'-x+1/2, -z+1/2, y'
'x+1/2, -z+1/2, -y'
'x+1/2, z+1/2, y'
'-x+1/2, z+1/2, -y'
'-z+1/2, -y+1/2, x'
'-z+1/2, y+1/2, -x'
'z+1/2, -y+1/2, -x'
'z+1/2, y+1/2, x'

_cell_length_a                   34.3966(2)
_cell_length_b                   34.3966(2)
_cell_length_c                   34.3966(2)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     40695.5(7)
_cell_formula_units_Z            8
_cell_measurement_reflns_used    6231
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      75.8300
_cell_measurement_theta_min      2.2150
_shelx_estimated_absorpt_T_max   0.981
_shelx_estimated_absorpt_T_min   0.915
_exptl_absorpt_coefficient_mu    0.647
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.86470
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
CrysAlisPro 1.171.42.63a (Rigaku Oxford Diffraction, 2022)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    0.326
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_F_000             4000
_exptl_crystal_size_max          0.14
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.03
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0210
_diffrn_reflns_av_unetI/netI     0.0168
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       40
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       38
_diffrn_reflns_limit_k_min       -40
_diffrn_reflns_limit_l_max       32
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            11527
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        66.571
_diffrn_reflns_theta_max         66.571
_diffrn_reflns_theta_min         2.225
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 10.0000
_diffrn_detector_type            HyPix
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_details      
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω   -116.00 -89.00   0.50   13.08    --  -47.78-128.00 -96.00   54
  2  ω    108.00 144.00   0.50  135.75    --  104.41 129.00  31.00   72
  3  ω    -25.00  26.00   0.50   13.08    --   46.53 -19.00-120.00  102
  4  ω    -67.00 -35.00   0.50  135.75    -- -105.66  61.00-180.00   64
  5  ω    -68.00 -39.00   0.50  135.75    -- -105.66  61.00  30.00   58
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  
'XtaLAB Synergy, Single source at home/near, HyPix'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type       
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0016457000
_diffrn_orient_matrix_UB_12      0.0445272000
_diffrn_orient_matrix_UB_13      0.0039634000
_diffrn_orient_matrix_UB_21      -0.0327152000
_diffrn_orient_matrix_UB_22      -0.0039354000
_diffrn_orient_matrix_UB_23      0.0303557000
_diffrn_orient_matrix_UB_31      0.0305994000
_diffrn_orient_matrix_UB_32      -0.0018137000
_diffrn_orient_matrix_UB_33      0.0327100000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54184
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'PhotonJet (Cu) X-ray Source'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                1566
_reflns_number_total             1824
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'CrysAlisPro 1.171.42.63a (Rigaku OD, 2022)'
_computing_data_collection       'CrysAlisPro 1.171.42.63a (Rigaku OD, 2022)'
_computing_data_reduction        'CrysAlisPro 1.171.42.63a (Rigaku OD, 2022)'
_computing_molecular_graphics    'Olex2 1.5-ac5-024 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5-ac5-024 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT  (Sheldrick, 2015)'
_refine_diff_density_max         0.156
_refine_diff_density_min         -0.202
_refine_diff_density_rms         0.026
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.014
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     41
_refine_ls_number_reflns         1824
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0265
_refine_ls_R_factor_gt           0.0247
_refine_ls_restrained_S_all      1.014
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0562P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0720
_refine_ls_wR_factor_ref         0.0734
_refine_special_details          
'Used  solvent mask to account electron denisty assoicated with disordered solvent molecules,SQUEEZE'
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
2. Others
 Fixed Sof: C4(0.5) H4(0.5) C3(0.5) H3(0.5)
3.a Aromatic/amide H refined with riding coordinates:
 C4(H4), C3(H3)
;
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Zn1 Zn 0.28264(2) 0.71736(2) 0.28264(2) 0.05071(12) Uani 1 6 d S T P . .
O1 O 0.250000 0.750000 0.250000 0.0479(4) Uani 1 24 d S T P . .
O2 O 0.27285(2) 0.66286(2) 0.27285(2) 0.0855(3) Uani 1 2 d S T P . .
C2 C 0.250000 0.60288(4) 0.250000 0.0881(5) Uani 1 4 d S T P . .
C1 C 0.250000 0.64620(4) 0.250000 0.0730(4) Uani 1 4 d S T P . .
C5 C 0.250000 0.52154(5) 0.250000 0.1114(8) Uani 1 4 d S T P . .
C4 C 0.23377(16) 0.54276(5) 0.21983(16) 0.125(3) Uani 0.5 1 d . . P A -1
H4 H 0.222556 0.529622 0.199023 0.151 Uiso 0.5 1 calc R U P A -1
C3 C 0.23381(12) 0.58247(5) 0.21987(12) 0.114(2) Uani 0.5 1 d . . P A -1
H3 H 0.222700 0.595832 0.199154 0.137 Uiso 0.5 1 calc R U P A -1


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Zn1 O1 1.9447(2) . ?
Zn1 O2 1.9342(8) 6_566 ?
Zn1 O2 1.9341(8) . ?
Zn1 O2 1.9342(8) 12_665 ?
O2 C1 1.2506(10) . ?
C2 C1 1.490(2) . ?
C2 C3 1.370(2) . ?
C5 C5 1.482(3) 145_565 ?
C5 C4 1.386(3) . ?
C4 C3 1.366(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Zn1 O1 111.01(3) . . ?
O2 Zn1 O1 111.01(3) 12_665 . ?
O2 Zn1 O1 111.01(3) 6_566 . ?
O2 Zn1 O2 107.89(3) . 12_665 ?
O2 Zn1 O2 107.89(3) . 6_566 ?
O2 Zn1 O2 107.89(3) 12_665 6_566 ?
Zn1 O1 Zn1 109.5 28_565 74_565 ?
Zn1 O1 Zn1 109.5 28_565 . ?
Zn1 O1 Zn1 109.5 51 74_565 ?
Zn1 O1 Zn1 109.5 74_565 . ?
Zn1 O1 Zn1 109.471(1) 51 28_565 ?
Zn1 O1 Zn1 109.471(1) 51 . ?
C1 O2 Zn1 131.53(8) . . ?
C3 C2 C1 120.83(10) . . ?
O2 C1 O2 125.46(13) 51 . ?
O2 C1 C2 117.27(7) . . ?
O2 C1 C2 117.27(7) 51 . ?
C4 C5 C5 121.77(11) . 145_565 ?
C3 C4 C5 121.7(2) . . ?
C4 C3 C2 120.9(2) . . ?

_smtbx_masks_special_details     
;
    A solvent mask was calculated and 5341 electrons were found in a void volume of 34843 angstroms cubed per unit cell, this is consistent with 13 hexane molecules.
;
loop_
_smtbx_masks_void_nr
_smtbx_masks_void_average_x
_smtbx_masks_void_average_y
_smtbx_masks_void_average_z
_smtbx_masks_void_volume
_smtbx_masks_void_count_electrons
_smtbx_masks_void_content
1 -0.956 -0.365 -0.977 34843.3 5340.8 ?

_smtbx_masks_void_probe_radius   1.2
_smtbx_masks_void_truncation_radius 1.2
_olex2_exptl_crystal_mounting_method 'Shard of crystal '
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details 
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.183
_oxdiff_exptl_absorpt_empirical_full_min 0.889


_chemical_properties_physical    Moisture-sensitive
